JOHN WILEY & SONS, INC.
This book is printed on acid-free paper.
Copyright 2011 by John Wiley & Sons, Inc. All rights reserved
Published by John Wiley & Sons, Inc., Hoboken, New Jersey
Published simultaneously in Canada
No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means,
electronic, mechanical, photocopying, recording, scanning, or otherwise, except as permitted under Section 107 or 108
of the 1976 United States Copyright Act, without either the prior written permission of the Publisher, or authorization
through payment of the appropriate per-copy fee to the Copyright Clearance Center, 222 Rosewood Drive, Danvers, MA
01923, (978) 750-8400, fax (978) 646-8600, or on the web at www.copyright.com. Requests to the Publisher for
permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street, Hoboken,
NJ 07030, (201) 748-6011, fax (201) 748-6008, or online at www.wiley.com/go/permissions.
Limit of Liability/Disclaimer of Warranty: While the publisher and the author have used their best efforts in preparing
this book, they make no representations or warranties with respect to the accuracy or completeness of the contents of
this book and speciﬁcally disclaim any implied warranties of merchantability or ﬁtness for a particular purpose. No
warranty may be created or extended by sales representatives or written sales materials. The advice and strategies
contained herein may not be suitable for your situation. You should consult with a professional where appropriate.
Neither the publisher nor the author shall be liable for any loss of proﬁt or any other commercial damages, including
but not limited to special, incidental, consequential, or other damages.
For general information about our other products and services, please contact our Customer Care Department within the
United States at (800) 762-2974, outside the United States at (317) 572-3993 or fax (317) 572-4002.
Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be
available in electronic books. For more information about Wiley products, visit our web site at www.wiley.com.
Library of Congress Cataloging-in-Publication Data:
Li, Zongjin, Dr.
Advanced concrete technology / Zongjin Li.
ISBN 978-0-470-43743-8 (cloth); ISBN 978-0-470-90239-4 (ebk); ISBN 978-0-470-90241-7 (ebk);
ISBN 978-0-470-90243-1 (ebk); ISBN 978-0-470-95006-7 (ebk); ISBN 978-0-470-95166-8 (ebk);
ISBN 978-0-470-95188-0 (ebk)
1. Concrete. I. Title.
Printed in the United States of America
10 9 8 7 6 5 4 3 2 1
To students, teachers, researchers, and engineers in the ﬁeld of concrete, who are the driving forces
for the development of the science and technology of concrete, including the personnel working
on the China 973 project, Basic Study on Environmentally Friendly Contemporary Concrete
Introduction to Concrete
Concrete Deﬁnition and Historical Development
Concrete as a Structural Material 7
Characteristics of Concrete 10
Types of Concrete 14
Factors Inﬂuencing Concrete Properties 16
Approaches to Study Concrete 19
Discussion Topics 21
Materials for Making Concrete
Discussion Topics 88
Workability of Fresh Concrete 94
Mix Design 107
Procedures for Concrete Mix Design 116
Manufacture of Concrete 122
Delivery of Concrete 123
Concrete Placing 125
Early-Age Properties of Concrete 135
Structure of Concrete
Structural Levels 141
Structure of Concrete in Nanometer Scale: C–S–H Structure
Transition Zone in Concrete 152
Microstructural Engineering 156
Discussion Topics 162
Strengths of Hardened Concrete 164
Stress–Strain Relationship and Constitutive Equations
Dimensional Stability—Shrinkage and Creep 197
Discussion Topics 246
Advanced Cementitious Composites
Fiber-Reinforced Cementitious Composites 251
High-Strength Cementitious Composites 270
Polymers in Concrete 281
Shrinkage-Compensating Concrete 292
Self-Compacting Concrete 296
Engineered Cementitious Composite 310
Tube-Reinforced Concrete 312
High-Volume Fly Ash Concrete 316
Structural Lightweight Concrete 317
Heavyweight Concrete 317
Discussion Topics 317
Concrete Fracture Mechanics
Linear Elastic Fracture Mechanics 330
The Crack Tip Plastic Zone 337
Crack Tip Opening Displacement 340
Fracture Process in Concrete 342
Nonlinear Fracture Mechanics for Concrete 346
Two-Parameter Fracture Model 348
Size Effect Model 355
The Fictitious Model by Hillerborg 364
R-Curve Method for Quasi-Brittle Materials 369
Nondestructive Testing in Concrete Engineering
Review of Wave Theory for a 1D Case 394
Reﬂected and Transmitted Waves 403
Attenuation and Scattering 406
Main Commonly Used NDT-CE Techniques 407
Noncontacting Resistivity Measurement Method 458
Discussion Topics 468
The Future and Development Trends of Concrete
Sustainability of Concrete 476
Deep Understanding of the Nature of Hydration 483
Load-Carrying Capability–Durability Uniﬁed Service Life Design
High Toughness and Ductile Concrete 487
Concrete is the most widely used material in the world. It plays an important role in infrastructure
and private buildings construction. Understanding the basic behaviors of concrete is essential for
civil engineering students to become civil engineering professionals. There have been some very
good books regarding concrete, including Concrete by Mindess, Young, and Darwin, Concrete:
Structure, Properties, and Materials by Mehta and Monteriro, and Concrete Technology by
Neville and Brook. The motivation to write this book is to introduce new methodologies, new
developments, and new innovations in concrete technology. The unique features of this book
include the introduction of end use guided research strategy for concrete, uniﬁcation of materials
and structures studies, and an emphasize on fundamental exploration of concrete structures,
state of art of concrete development, and innovations. This book provides more comprehensive
knowledge on concrete technology, including the systematic introduction of concrete fracture
mechanics and nondestructive evaluation for concrete engineering.
The book is divided into nine chapters. Chapter 1 gives a brief introduction of concrete,
including its historic development and advantages. Chapter 2 provides the knowledge of raw
materials used for making concrete, covering aggregates, binders, admixtures, and water. Chapter
3 discusses the properties of fresh concrete, including workability and the corresponding measurement methods. Chapter 4 focuses on the structure of concrete at different scales, especially
the calcium silicate hydrate at nanometer scale. Chapter 5 covers the properties of hardened
concrete, including strength, durability, stress–strain relation, and dimension stability. Chapter 6
provides updated knowledge on various cement-based composites, including self-consolidation
concrete, ultra-high-strength concrete, and extruded and engineered cementitious composites.
Chapter 7 focuses the fracture behavior of concrete and provides the basic knowledge of fracture mechanics of concrete. Chapter 8 covers the essential knowledge of nondestructive testing
of concrete engineering, including wave propagation theory in 1-D case, detecting principles of
different NDT methodologies and techniques of different NDT methods. In Chapter 9, the issues
regarding the future and development trend of concrete have been discussed.
Although the book is designed and written primarily to meet the teaching needs for undergraduate students at senior level and graduate students at entry level, it can serve as a reference
or a guide for professional engineers in their practice.
In the process of writing this book, the authors received enthusiastic help and invaluable
assistance from many people, which is deeply appreciated. The authors would like to express
his special thanks to Dr. Garrison C. K. Chau, Dr. Biwan Xu, and Dr. Jianzhong Shen for their
help in editing the book draft. Mr. Mike Pomfret is acknowledged for his professional page
proofreading. The photos provided by Profs. Wei Sun, Tongbo Sui, Linhai Han, and Zhen He;
Drs. Xiaojian Gao, Herbert Zheng, and Jinyang Jiang; Mr. Peter Allen; and the companies of
Ove Arup and Gammon are greatly appreciated.
The support from China Basic Research Grant, Basic Research on Environmentally Friendly
Contemporary Concrete (2009CB623200) is greatly acknowledged.
Finally, I would like to thank for my wife, Xiuming Cui, my daughters Yexin Li and Aileen
Li for their love, understanding, and support.
INTRODUCTION TO CONCRETE
CONCRETE DEFINITION AND HISTORICAL DEVELOPMENT
Concrete is a manmade building material that looks like stone. The word “concrete” is derived
from the Latin concretus, meaning “to grow together.” Concrete is a composite material composed of coarse granular material (the aggregate or ﬁller) embedded in a hard matrix of material
(the cement or binder) that ﬁlls the space among the aggregate particles and glues them together.
Alternatively, we can say that concrete is a composite material that consists essentially of a binding medium in which are embedded particles or fragments of aggregates. The simplest deﬁnition
of concrete can be written as
concrete = ﬁller + binder
Depending on what kind of binder is used, concrete can be named in different ways. For
instance, if a concrete in made with nonhydraulic cement, it is called nonhydraulic cement
concrete; if a concrete made of hydraulic cement, it is called hydraulic cement concrete; if a
concrete is made of asphalt, it is called asphalt concrete; if a concrete is made of polymer, it
is called polymer concrete. Both nonhydraulic and hydraulic cement need water to mix in and
react. They differ here in the ability to gain strength in water. Nonhydraulic cement cannot gain
strength in water, while hydraulic cement does.
Nonhydraulic cement concretes are the oldest used in human history. As early as around
6500 bc, nonhydraulic cement concretes were used by the Syrians and spread through Egypt, the
Middle East, Crete, Cyprus, and ancient Greece. However, it was the Romans who reﬁned the
mixture’s use. The nonhydraulic cements used at that time were gypsum and lime. The Romans
used a primal mix for their concrete. It consisted of small pieces of gravel and coarse sand mixed
with hot lime and water, and sometimes even animal blood. The Romans were known to have
made wide usage of concrete for building roads. It is interesting to learn that they built some 5300
miles of roads using concrete. Concrete is a very strong building material. Historical evidence
also points out that the Romans used pozzalana, animal fat, milk, and blood as admixtures for
building concrete. To trim down shrinkage, they were known to have used horsehair. Historical
evidence shows that the Assyrians and Babylonians used clay as the bonding material. Lime was
obtained by calcining limestone with a reaction of
CaCO3 −−−−−→ CaO + CO2
When CaO is mixed with water, it can react with water to form
CaO + H2 O −−−−−−−−−−−−→ Ca (OH)2
Chapter 1 Introduction to Concrete
and is then further reacted with CO2 to form limestone again:
Ca (OH)2 + CO2 + H2 O −−−−−−−−−−−−→ CaCO3 + 2H2 O
The Egyptians used gypsum mortar in construction, and the gypsum was obtained by calcining
impure gypsum with a reaction of
2CaSO4 · H2 O −−−−−−−→ 2CaSO4 · 12 H2 O + 3H2 O
When mixed with water, half-water gypsum could turn into two-water gypsum and gain strength:
2CaSO4 · 12 H2 O + 3H2 O −−−−−−−−−−−−→ 2CaSO4 · 2H2 O
The Egyptians used gypsum instead of lime because it could be calcined at much lower
temperatures. As early as about 3000 bc, the Egyptians used gypsum mortar in the construction
of the Pyramid of Cheops. However, this pyramid was looted long before archeologists knew
about the building materials used. Figure 1-1 shows a pyramid in Gaza. The Chinese also used
lime mortar to build the Great Wall in the Qin dynasty (220 bc) (see Figure 1-2).
A hydraulic lime was developed by the Greeks and Romans using limestone containing
argillaceous (clayey) impurities. The Greeks even used volcanic ash from the island of Santorin,
while the Romans utilized volcanic ash from the Bay of Naples to mix with lime to produce
hydraulic lime. It was found that mortar made of such hydraulic lime could resist water. Thus,
hydraulic lime mortars were used extensively for hydraulic structures from second half of the
ﬁrst century bc to the second century ad However, the quality of cementing materials declined
throughout the Middle Ages. The art of burning lime was almost lost and siliceous impurities
were not added. High-quality mortars disappeared for a long period. In 1756, John Smeaton
Figure 1-1 Pyramid built with gypsum mortar in Gaza, Egypt
1.1 Concrete Deﬁnition and Historical Development
Figure 1-2 The Great Wall, built in the Qin dynasty
was commissioned to rebuild the Eddystone Light house off the coast of Cornwall, England.
Realizing the function of siliceous impurities in resisting water, Smeaton conducted extensive
experiments with different limes and pozzolans, and found that limestone with a high proportion
of clayey materials produced the best hydraulic lime for mortar to be used in water. Eventually,
Smeaton used a mortar prepared from a hydraulic lime mixed with pozzolan imported from Italy.
He made concrete by mixing coarse aggregate (pebbles) and powdered brick and mixed it with
cement, very close to the proportions of modern concrete. The rebuilt Eddystone Lighthouse
lasted for 126 years until it was replaced with a modern structure.
After Smeaton’s work, development of hydraulic cement proceeded quickly James Parker
of England ﬁled a patent in 1796 for a natural hydraulic cement made by calcining nodules of
impure limestone containing clay. Vicat of France produced artiﬁcial hydraulic lime by calcining
synthetic mixtures of limestone and clay. Portland cement was invented by Joseph Aspdin
of England. The name Portland was coined by Aspdin because the color of the cement after
hydration was similar to that of limestone quarried in Portland, a town in southern England.
Portland cement was prepared by calcining ﬁnely ground limestone, mixing it with ﬁnely divided
clay, and calcining the mixture again in a kiln until the CO2 was driven off. This mixture was
then ﬁnely ground and used as cement. However, the temperature claimed in Aspdin’s invention
was not high enough to produce true Portland cement. It was Isaac Johnson who ﬁrst burned the
raw materials to the clinkering temperature in 1845 to produce modern Portland cement. After
that, the application of Portland cement spread quickly throughout Europe and North America.
The main application of Portland cement is to make concrete. It was in Germany that the ﬁrst
systematic testing of concrete took place in 1836. The test measured the tensile and compressive
strength of concrete. Aggregates are another main ingredient of concrete, and which include sand,
crushed stone, clay, gravel, slag, and shale. Plain concrete made of Portland cement and aggregate
is usually called the ﬁrst generation of concrete. The second generation of concrete refers to
steel bar-reinforced concrete. Franc¸ois Coignet was a pioneer in the development of reinforced
concrete. (Day and McNeil, 1996). Coignet started experimenting with iron-reinforced concrete
in 1852 and was the ﬁrst builder ever to use this technique as a building material (Encyclopaedia
Chapter 1 Introduction to Concrete
Britannica, 1991). He decided, as a publicity stunt and to promote his cement business, to build a
house made of b´eton arm´e , a type of reinforced concrete. In 1853, he built the ﬁrst iron-reinforced
concrete structure anywhere; a four-story house at 72 Rue Charles Michels (Sutherland et al.,
2001). This location was near his family cement plant in St. Denis, a commune in the northern
suburbs of Paris. The house was designed by local architect Theodore Lachez (Collins, 2004).
Coignet had an exhibit at the 1855 Paris Exposition to show his technique of reinforced
concrete. At the exhibit, he forecast that the technique would replace stone as a means of
construction. In 1856 he patented a technique of reinforced concrete using iron tirants. In 1861
he put out a publication on his techniques.
Reinforced concrete was further developed by Hennebique at the end of the 19th century,
and it was realized that performance could be improved if the bars could be placed in tension,
thus keeping the concrete in compression. Early attempts worked, with the beams showing a
reduced tendency to crack in tension, but after a few months the cracks reopened. A good
description of this early work is given in Leonhardt (1964). The ﬁrst reinforced concrete bridge
was built in 1889 in the Golden Gate Park in San Francisco, California.
To overcome the cracking problem in reinforced concrete, prestressed concrete was developed and was ﬁrst patented by a San Francisco engineer as early as 1886. Prestressed means
that the stress is generated in a structural member before it carries the service load. Prestressed
concrete was referred to as the third generation of concrete. Prestressing is usually generated
by the stretched reinforcing steel in a structural member. According to the sequence of concrete
casting, prestressing can be classiﬁed as pretensioning or post-tensioning. Pretensioning pulls
the reinforcing steel before casting the concrete and prestress is added through the bond built
up between the stretched reinforcing steel and the hardened concrete. In the post-tensioning
technique, the reinforcing steel or tendon is stretched after concrete casting and the gaining
of sufﬁcient strength. In post-tensioning, steel tendons are positioned in the concrete specimen
through prereserved holes. The prestress is added to the member through the end anchorage.
Figure 1-3 shows the sequence of the pretensioning technique for prestressed concrete.
Prestressed concrete became an accepted building material in Europe after World War II,
partly due to the shortage of steel. North America’s ﬁrst prestressed concrete structure, the Walnut
(1) Pre-stress rebar
(2) Cast concrete
(3) Release rebar
Figure 1-3 Pretensioning sequence for prestressing concrete
1.1 Concrete Deﬁnition and Historical Development
Lane Memorial Bridge in Philadelphia, Pennsylvania, was completed in 1951. Nowadays, with
the development of prestressed concrete, long-span bridges, tall buildings, and ocean structures
have been constructed. The Barrios de Lura Bridge in Spain is currently the longest-span prestressed concrete, cable-stayed bridge in the world, with a main span of 440 m. In Canada, the
prestressed Toronto CN tower reaches a height of 553 m.
As a structural material, the compressive strength at an age of 28 days is the main design
index for concrete. There are several reasons for choosing compressive strength as the representative index. First, concrete is used in a structure mainly to resist the compression force. Second,
the measurement of compressive strength is relatively easier. Finally, it is thought that other properties of concrete can be related to its compressive strength through the microstructure. Pursuing
high compressive strength has been an important direction of concrete development. As early as
1918, Duff Adams found that the compressive strength of a concrete was inversely proportional
to the water-to-cement ratio. Hence, a high compressive strength could be achieved by reducing
the w /c ratio. However, to keep a concrete workable, there is a minimum requirement on the
amount of water; hence, the w /c ratio reduction is limited, unless other measures are provided to
improve concrete’s workability. For this reason, progress in achieving high compressive strength
was very slow before the 1960s. At that time, concrete with a compressive strength of 30 MPa
was regarded as high-strength concrete. Since the 1960s, the development of high-strength concrete has made signiﬁcant progress due to two main factors: the invention of water-reducing
admixtures and the incorporation of mineral admixtures, such as silica fume, ﬂy ash, and slag.
Water-reducing admixture is a chemical admixture that can help concrete keep good workability
under a very low w /c ratio; the latter are ﬁner mineral particles that can react with a hydration
product in concrete, calcium hydroxide, to make concrete microstructure denser. Silica fume also
has a packing effect to further improve the matrix density. In 1972, the ﬁrst 52-MPa concrete
was produced in Chicago for the 52-story Mid-Continental Plaza. In 1972, a 62-MPa concrete
was produced, also in Chicago, for Water Tower Place, a 74-story concrete building, the tallest in
the world at that time (see Figure 1-4). In the 1980s, the industry was able to produce a 95-MPa
concrete to supply to the 225 West Whacker Drive building project in Chicago, as shown in
Figure 1-5. The highest compressive strength of 130 MPa was realized in a 220-m-high, 58-story
building, the Union Plaza constructed in Seattle, Washington (Caldarone, 2009).
Concrete produced after the 1980s usually contains a sufﬁcient amount of ﬂy ash, slag,
or silica fume as well as many different chemical admixtures, so its hydration mechanism,
hydration products, and other microstructure characteristics are very different from the concrete
produced without these admixtures. Moreover, the mechanical properties are also different from
the conventional concrete; hence, such concretes are referred to as contemporary concretes.
There have been two innovative developments in contemporary concrete: self-compacting
concrete (SCC) and ultra-high-performance concrete (UHPC). SCC is a type of high-performance
concrete. High-performance concrete is a concept developed in the 1980s. It is deﬁned as a
concrete that can meet special performance and uniformity requirements, which cannot always
be achieved routinely by using only conventional materials and normal mixing, placing, and
curing practices. The requirements may involve enhancement of the characteristics of concrete,
such as placement and compaction without segregation, long-term mechanical properties, higher
early-age strength, better toughness, higher volume stability, or longer service life in severe
Self-compacting concrete is a typical example of high-performance concrete that can ﬁll
in formwork in a compacted manner without the need of mechanical vibration. SCC was initially developed by Professor Okamura and his students in Japan in the late 1980s (Ozama et al.,
1989). At that time, concrete construction was blooming everywhere in Japan. Since Japan is in an
Chapter 1 Introduction to Concrete
Water Tower Place in Chicago, Illinois, USA (Photo provided by Xiaojian
earthquake zone, concrete structures are usually heavily reinforced, especially at beam–column
joints. Hence, due to low ﬂowability, conventional concrete could hardly ﬂow past the heavy
reinforced rebars, leaving poor-quality cast concrete and leading to poor durability. Sometimes,
the reinforcing steel was exposed to air immediately after demolding. To solve the problem, Professor Okamura and his students conducted research to develop a concrete with high ﬂowability.
With the help of the invention of the high-range water reducer or plasticizer, such a concrete
was ﬁnally developed. They were so excited that they called this concrete “high-performance
concrete” at the beginning. It was corrected later on to SCC, as HPC covers broader meanings.
Durability is a main requirement of HPC. It has been found that many concrete structures could
not fulﬁll the service requirement, due not to lack of strength, but to lack of durability. For this
reason, concrete with high performance to meet the requirement of prolonging concrete service
life was greatly needed.
In the 1990s, a new “concrete” with a compressive concrete strength higher than 200 MPa
was developed in France. Due to the large amount of silica fume incorporated in such a material, it was initially called reactive powder concrete and later on changed to ultra-high-strength
(performance) concrete (UHSC), due to its extremely high compressive strength (Richard and
Cheyrezy, 1995). The ultra-high-strength concrete has reached a compressive strength of 800 MPa
1.2 Concrete as a Structural Material
Figure 1-5 The 225 West Whacker Drive building in Chicago, Illinois, USA (Photo
provided by Xiaojian Gao)
with heating treatment. However, it is very brittle, hence, incorporating ﬁbers into UHSC is necessary. After incorporating ﬁne steel ﬁbers, ﬂexural strength of 50 MPa can be reached. The ﬁrst
trial application of UHSC was a footbridge built in Sherbrooke, Canada (Aitcin et al., 1998).
CONCRETE AS A STRUCTURAL MATERIAL
In this book, the term concrete usually refers to Portland cement concrete, if not otherwise
speciﬁed. For this kind of concrete, the compositions can be listed as follows:
+ water (& admixtures) → cement paste
+ ﬁne aggregate → mortar
+ coarse aggregate → concrete
Here we should indicate that admixtures are almost always used in modern practice and
thus have become an essential component of contemporary concrete. Admixtures are deﬁned as
Chapter 1 Introduction to Concrete
materials other than aggregate (ﬁne and coarse), water, and cement that are added into a concrete
batch immediately before or during mixing. The use of admixtures is widespread mainly because
many beneﬁts can be achieved by their application. For instance, chemical admixtures can modify
the setting and hardening characteristics of cement paste by inﬂuencing the rate of cement
hydration. Water-reducing admixtures can plasticize fresh concrete mixtures by reducing surface
tension of the water. Air-entraining admixtures can improve the durability of concrete, and
mineral admixtures such as pozzolans (materials containing reactive silica) can reduce thermal
cracking. A detailed description of admixtures is given in Chapter 2.
Concrete is the most widely used construction material in the world, and its popularity can
be attributed to two aspects. First, concrete is used for many different structures, such as dams,
pavements, building frames, or bridges, much more than any other construction material. Second,
the amount of concrete used is much more than any other material. Its worldwide production
exceeds that of steel by a factor of 10 in tonnage and by more than a factor of 30 in volume.
In a concrete structure, there are two commonly used structural materials: concrete and
steel. A structural material is a material that carries not only its self-weight, but also the load
passing from other members.
Steel is manufactured under carefully controlled conditions, always in a highly sophisticated
plant; the properties of every type of steel are determined in a laboratory and described in a
manufacturer’s certiﬁcate. Thus, the designer of a steel structure need only specify the steel
complying with a relevant standard, and the constructor needs only to ensure that the correct
steel is used and that connections between the individual steel members are properly executed
(Neville and Brooks, 1993).
On the other hand, concrete is produced in a cruder way and its quality varies considerably.
Even the quality of cement, the binder of concrete, is guaranteed by the manufacturer in a manner
similar to that of steel; however, the quality of concrete is hardly guaranteed because of many
other factors, such as aggregates, mixing procedures, and skills of the operators of concrete
production, placement, and consolidation.
It is possible to obtain concrete of speciﬁed quality from a ready-mix supplier, but, even in
this case, it is only the raw materials that are bought for a construction job. Transporting, placing,
and, above all, compacting greatly inﬂuence the quality of cast concrete structure. Moreover,
unlike the case of steel, the choice of concrete mixes is virtually inﬁnite and therefore the
selection has to be made with a sound knowledge of the properties and behavior of concrete.
It is thus the competence of the designer and speciﬁer that determines the potential qualities of
concrete, and the competence of the supplier and the contractor that controls the actual quality
of concrete in the ﬁnished structure. It follows that they must be thoroughly conversant with the
properties of concrete and with concrete making and placing.
In a concrete structure, concretes mainly carry the compressive force and shear force, while
the steel carries the tension force. Moreover, concrete usually provides stiffness for structures to
keep them stable.
Concretes have been widely used to build various structures. High-strength concrete has
been used in many tall building constructions. In Hong Kong, grade 80 concrete (80 MPa) was
utilized in the columns of the tallest building in the region. As shown in Figure 1-6, the 88-story
International Finance Centre was built in 2003 and stands 415 m (1362 ft) tall.
Concrete has also been used in bridge construction. Figure 1-7 shows the recently built
Sutong Bridge that spans the Yangtze River in China between Nantong and Changshu, a satellite
city of Suzhou, in Jiangsu province. It is a cable-stayed bridge with the longest main span, 1088
meters, in the world. Its two side spans are 300 m (984 ft) each, and there are also four small
1.2 Concrete as a Structural Material
Figure 1-6 International Finance Center, Hong Kong (Photo courtesy of user WiNG on
Wikimedia Commons, http://commons.wikimedia.org/wiki/File:HK_ifc_Overview.jpg)
Figure 1-7 The Sutong Bridge in Suzhou, Jiangsu, China
Chapter 1 Introduction to Concrete
Three Gorges Dam, Hubei, China
Dams are other popular application ﬁelds for concrete. The ﬁrst major concrete dams, the
Hoover Dam and the Grand Coulee Dam, were built in the 1930s and they are still standing.
The largest dam ever built is the Three Gorges Dam in Hubei province, China, as shown in
Figure 1-8. The total concrete used for the dam was over 22 million m3 .
Concrete has also been used to build high-speed railways. Shinkansen, the world’s ﬁrst
contemporary high-volume (initially 12-car maximum), “high-speed rail,” was built in Japan
in 1964. In Europe, high-speed rail was introduce during the International Transport Fair in
Munich in June 1965. Nowadays, high-speed rail construction is blooming in China. According
to planning, 17,000 km of high-speed rail will be built in China by 2012. Figure 1-9 shows a
high-speed rail system in China.
In addition, concrete has been widely applied in the construction of airport runways, tunnels,
highways, pipelines, and oil platforms. As of now, the annual world consumption of concrete
has reached a value such that if concrete were edible, every person on earth would have 2000 kg
per year to “eat.” You may wonder why concrete has become so popular.
CHARACTERISTICS OF CONCRETE
1.3.1 Advantages of concrete
(a) Economical : Concrete is the most inexpensive and the most readily available material
in the world. The cost of production of concrete is low compared with other engineered
construction materials. The three major components in concrete are water, aggregate, and
cement. Compared with steels, plastics, and polymers, these components are the most
inexpensive, and are available in every corner of the world. This enables concrete to be
produced worldwide at very low cost for local markets, thus avoiding the transport expenses
necessary for most other materials.